# Constitutive laws for transport of water, vapour and chloride

In document FIB-42 (Page 120-133)

## 9 Transport of water, vapour and chloride in hardened concrete

### 9.3 Constitutive laws for transport of water, vapour and chloride

A general relationship for transport of water in concrete exists [Persson 1992)]:

m = -2.911·P(cap)p2 + 0.3783·P(cap)p + 0.533 {R2 = 0.91} (9-1) where

m = t/h² the resistance to capillary suction (s/m²) t time (s)

h penetration depth (0.005 < h < 0.03 m)

For vapour transport of mature HPC the following correlation was found [Persson (1992)]:

δc = (97.4·(RH) - 59)·(w/c)² - (66.6·(RH) - 41.5)·w/c +14.2·(RH) - 9.7 (9-2) where

w/c denotes the water-cement ratio (0.25 < w/c < 0.50) RH denotes the relative humidity (0.90 < RH < 0.95) δc denotes the vapour permeability of HPC (x106 m²/s)

The vapour permeability of mature HPC seems to have a minimum at w/c ≈ 0.30. The reason for this may be compaction problems at w/c < ≈ 0.30. At larger depth of the concrete, especially of HPC, the water transport is more or less prohibited by internal forces mainly due to autogenous shrinkage [Persson (1997, 1997a)]. Even after 13 years of water curing concrete did not obtain saturation, Figure 9-6. Long-term RH in 1 m diameter concrete columns was correlated in the following way [Persson (1996)]:

RHA = 0.91·(w/c) 0.2322 {R2 = 0.93} (9-3)

RHS = 0.96·(w/c) 0.1989 {R2 = 0.82} (9-4)

RHW = 0.84·(w/c)-0.0152 {R2 = 0.52} (9-5)

where

A denotes air curing

RH denotes long-term RH in 1 m diameter columns after 13 years S denotes sealed curing

W denotes water curing

The following equation for the chloride migration coefficient, D, is based on studies on concretes with a low-alkali CEM I 42.5 BV/SR/LA cement (C3A = 1.7 % and C4AF = 13 %), typical for HPC production [Persson (2001)]:

D={[(0.0055·ln(t)–0.2122)·c–3.5·ln(t)+104]·(4·w/b-1.2)/0.4}·(10-12) {R²=0.88} (9-6) where

c denotes the cement content (375 < c < 450 kg/m³) D denotes D (⋅10-12 m2/s)

ln(t) denotes the natural logarithm of concrete age (1 < t < 36 months) w/b denotes the water-binder ratio, 1:1 (0.35 < w/b < 0.50)

The following equation was obtained for the Pozzolan interaction between Portland cement and additions of silica fume, fly ash and slag as regards D [Boubitsas (2000), CTH Nordtest 492, Tang (2000), Persson (2001, 2001a)]:

ceq. = c + 0.2·fl + 1.6·sf + 1.0·sl {R2 = 0,81} (9-7) where

ceq. denotes the equivalent amount of cement to be used in equation (9-6) fl denotes the amount of fly ash (0.1 < (fl/c) < 0.25)

sf denotes the amount of silica fume (0.05 < (sf/c) < 0.12) sl denotes the amount of slag (0 < (sl/c) < 0.70)

0.00 0.50 1.00 1.50

0.20 0.30 0.40 0.50

Water-binder ratio, w/b Vapour permeability (x10^6 m²/s)

Mature-RF=0.85 Mature-RF=0.90 Mature-RF=0.95 Young-RF=0.85 Young-RF=0.90 Young-RF=0.95

0.60 0.70 0.80 0.90 1.00

0.20 0.30 0.40 0.50 0.60

Water-cement ratio

Relative humidity, RH

A As S Ss W Ws

Fig. 9-5: The vapour permeability of mature and young HPC at varying w/c and RH

Fig. 9-6: Long-term RH in 1 m concrete columns versus w/c. s = 10% silica fume, A = air curing, S = sealed, W = water

9.4 Conclusions

Constitutive laws for estimating the transport of water, vapour and chloride in Portland cement based systems were outlined. The diffusivity, permeability and capillary conditions of concrete were modelled. HPC generally exhibited lower water and chloride transport coefficients than normal concrete. For vapour transport a minimum transport coefficient seems to exist at w/c ≈ 0.30 (thus increasing at lower and larger w/c than 0.30).

### References

ACI - American Concrete Institute: ACI 03.95 – R8860, State-of-the-Art Report on Dynamic Fracture, ACI Committee 446, 1995.

ACI - American Concrete Institute: ACI 209.3R-XX, Time Dependent Effects in Concrete Structures, Reported by ACI Committee 209, M. A. Chiorino and W. Dilger Editors, Draft November 2007 Ahlgren, L., Bergström, S. G., Fagerlund, G., Nilsson, L.-O.: Moisture binding in Porous Building

Materials, Report 36, Div. of Building Physics, Lund Institute of Technology, Lund, 1972.

Al-Kubaisy, M.A., Young A.G.: Failure of concrete under sustained tension. Magazine of Concrete Research, Vol. 27, 1975, 171-178.

Alliche, A., Francois, D.: Damage of Concrete in Fatigue. ASCE Journal of Engineering Mechanics, Vol. 118, No. 11, 1992.

Alonso Junghanns, M.T.: Zur Risssicherheit zementgebundener dehnungsbehinderter Schichten unter Berücksichtigung von Dauereinflüssen. Dissertation, TU Hamburg-Harburg, Shaker Verlag, Aachen 1998.

Altoubat, S.A., Lange, D.A.: Tensile basic creep: Measurements and behaviour at early age. ACI Materials Journal Vol. 98 No. 5, September-October 2001, pp. 386-393.

Altoubat, S.A., Lange, D.A.: The Pickett effect at early age and experiment separating its mechanisms in tension. Materials and Structures / Matériaux et Constructions, Vol. 35, May 2002, 211-218.

ASTM E 104-85: Standard Practice for Maintaining Constant RH by Means of Aqueous Solutions.

ASTM. Philadelphia, 1985, pp. 33-34, 637.

Bache, H.H.: Densified Cement/Ultra-fine Particle-Based Materials. 2. International Conference on Superplasticizers in Concrete, Ottawa, 1981; also published by Aalborg Portland-Cement-Fabrik, DK-9100 Aalborg Denmark, pp. 1-35.

Barpi, F., Ferrara, G., Imperato, L., Valente, S.: Lifetime of concrete dam models under constant loads. Materials and Structures / Matériaux et Constructions, Vol. 32, March 1999, 103-111.

Bažant Z.P. (1972a): “Numerical Determination of Long-range Stress History from Strain History in Concrete”, Materials and Structures, Vol. 5, 1972, pp. 135-141.

Bažant, Z.P. (1972b): “Prediction of Concrete Creep Effects Using Age-adjusted Effective Modulus Method”, Journal of the American Concrete Institute, V. 69, 1972, pp. 212-217.

Bazant, Z.P., Kazemi, M. T., Hasegawa, T., Mazars, J.: Size effect in Brazilian split-cylinder test:

measurements and fracture analysis. ACI Materials Journal, Vol. 88, No. 3, 1991, pp. 325-332.

Bažant, Z.P., Schell, W.F.: Fatigue Fracture of High-Strength Concrete and Size-Effect. ACI Materials Journal, Vol. 90, No. 5, 1993.

Bergner, H.: Rissbreitenbeschränkung zwangbeanspruchter Bauteile aus hochfestem Normalbeton.

Deutscher Ausschuss für Stahlbeton, Heft 482, Beuth Verlag GmbH, Berlin, Wien, Zürich, 1997.

Bissonnette, B., Pigeon, M.: Tensile creep at the early ages of ordinary, silica fume and fiber reinforced concretes. Cement and Concrete Research Vol. 25, No. 5, 1995, pp. 1075-1085.

Bissonnette, B., Pigeon, M.: Viscoelastic behaviour of concrete in tension and dimensional compatibility of concrete repairs. Materials and Structures / Matériaux et Constructions, Vol. 33, March 2000, 108-118.

Blaschke, F., Losekamp, Ch., Mehlhorn, G.: Zugtragvermögen nach lang andauernder statischer sowie schwellender Zugvorbelastung von Beton. Forschungsbericht Nr. 20 aus dem Fachgebiet Massivbau der Gesamthochschule Kassel, 1993.

Boubitsas, D., Paulou, K.: SCC for Marine Environment, TVBM-5048, Lund Institute of Technology, Lund, 2000, 55 pp.

Buyukozturk, O., Tseng, T.-M.: Concrete in Biaxial Cyclic Compression. ASCE Journal of Structural Engineering, Vol. 110, Nr. 3, 1984.

Carino, N. J., Tank, R. C.: Maturity functions for concrete made with various cements and admixtures.

In: Testing During Construction, Proceedings o f an International RILEM Workshop, Chapman and Hall, 1990, pp. 192-206.

Carpinteri, A., Valente, S., Zhou, F.P., Ferrara, G., Melchiorri, G.: Tensile and flexural creep rupture tests on partially damaged concrete specimens. RILEM Materials and Structures, Vol. 30, 1997, 269-276.

Carrasquillo, P. M., Carrasquillo, R. L.: Evaluation of the use of current concrete practice in the production of high strength concrete. ACI Materials Journal, Vol. 78, No. 14, 1981, pp. 171-178.

Carrasquillo, R. L., Nilson, A. H., Slate, F. O.: Properties of high strength concrete subjected to short-term loads. ACI Journal, May-June 1981, pp. 171-178.

CEB – Comité Euro-international du Béton: CEB Design Manual on Structural Effects of Time-dependent Behaviour of Concrete, M. A. Chiorino Chairman of Editorial Team, CEB Bulletin d’Information No. 142-142 Bis, March 1984.

CEB – Comité Euro-international du Béton: State of the Art Report, Fatigue of Concrete Structures.

CEB Bulletin D'Information, No. 188, 1988.

CEB – Comité Euro-international du Béton: State of the Art Report, High Strength Concrete. CEB Bulletin d'Information, No. 197, 1990.

CEB – Comité Euro-international du Béton: Evaluation of the time dependent behavior of concrete.

CEB Bulletin d'Information, No. 199, 1990.

CEB – Comité Euro-international du Béton: Revision of the design aids of the CEB Design Manual Structural Effects of Time-dependent Behaviour of Concrete in accordance with the CEB-FIP Model Code 1990, (principal authors M. A. Chiorino and G. Lacidogna), CEB Bulletin d'Information, No. 215, 1993.

CEB – Comité Euro-international du Béton: CEB-FIP Model Code 1990, Bulletin d’Information, No.

213/214, Thomas Telford Ltd., London, 1993.

CEB – Comité Euro-international du Béton: State of the Art Report, High Performance Concrete, Recommended Extensions to the Model Code 90, Research Needs. CEB Bulletin d'Information, No. 228, 1995.

Cetin, A., Carrasquillo, R. L.: High-performance concrete: Influence of coarse aggregates on mechanical properties, ACI Materials Journal, technical paper, title No. 95-M24, May-June 1998, pp. 252-261.

Chiorino M.A.: A Rational Approach to the Analysis of Creep Structural Effects, in: J. Gardner and J.

Weiss Editors, Shrinkage and Creep of Concrete, ACI American Concrete Institute SP-227, 2005, pp. 107-141.

Cook, J. E.: 10,000 psi concrete. Concrete International, Vol. 11, No. 10, 1989, pp. 67-75.

CTH Rapid Test for Determination of D in Concrete, NT BUILD 492, 2000.

Dahl, K.: A Constitutive Model for Normal and High Strength Concrete. Dissertation, Danmarks Tekniske Højskole, Lynhby, 1992.

Dargel, H. J.: Zur rechnerischen Analyse von Stahlbetontragwerken unter stoßartiger Beanspruchung.

de Larrard, F., Acker, P.: Creep in high and very high performance concrete. High Performance Concrete - From material to structure, edited by Y. Malier, E & FN Spon, Paris, 1992, pp. 115-126.

Dettling, H.: Die Wärmedehnung des Zementsteins, der Gesteine und der Betone. Schriftenreihe des Otto-Graf-Instituts der Technischen Hochschule Stuttgart, No. 3, Stuttgart, 1962.

Dilger, W. (1998): Private communication, 1998.

Dilger, W. H. et al.: Shrinkage and creep of high-performance concrete (HPC). Proceedings Adam Neville Symposium on Concrete Technology, Las Vegas Nev. USA, V. M. Malhotra (ed.), CANMET, June 1995, pp. 59-84.

DIN 1048-5: Prüfverfahren für Beton, Festbeton, gesondert hergestellte Probekörper, Juni 1991.

Dipartimento di Ingegneria Strutturale e Geotecnica, Politecnico di Torino:

www.polito.it/creepanalysis, 2004-2007

Duda, H.: Fracture Mechanical Behaviour of Concrete under Monotonic and Cyclic Tensile Loading (in German). Deutscher Ausschuss für Stahlbeton, Heft 419, Beuth Verlag, Berlin, 1991.

EN 12394 [1996]: Testing Concrete - Determination of Compressive Strength of Test Sprecimen.

1996.

ENV 1992-1 (1991), European Committee for Standardization (CEN), ENV 1992-1, Design of Concrete Structures. Part 1: General rules and rules for buildings, 1991.

Fagerlund, G.: Influence of Environmental Factors on the Frost Resistance of Concrete, TVBM-3059, Lund Institute of Technology, Lund, 1994, pp. 19-22.

Fagerlund, G.: The Critical Degree of Saturation Procedure - A General Procedure of Estimating the Frost Resistance of Materials and Structures, Report Fo 12:76, The Cement and Concrete Research Institute, Stockholm, 1976.

Franke, L.: Schadensakkumulation und Restfestigkeit im Licht der Bruchmechanik. Fortschritte im konstruktiven Ingenieurbau, Gallus Rehm zum 60. Geburtstag, Ernst & Sohn, Berlin 1984, pp.

187-197.

Frénaij, J.: Time dependent shear transfer in cracked reinforced concrete. Dissertation, TU Delft 1989.

Gardner, N. J., Zhao, J. W.: Creep and shrinkage revisited. ACI Materials Journal, Vol. 90, No. 3, 1993, pp. 236-246.

Giaccio, G., Rocco, C., Zerbino, R.: The fracture energy (GF) of high-strength concretes. Materials and Structures, Vol. 26, 1993, pp. 381-386.

Gopalaratnam, V.S., Shah, S.P.: Softening Response of Plain Concrete in Direct Tension. ACI Journal, Vol. 82, No. 27, 1985.

Grimm, R.: Einfluss bruchmechanischer Kenngrößen auf das Biege- und Schubtragverhalten hochfester Betone. Doctoral thesis, Technical University of Darmstadt, Civil Engineering, 1996.

Guénot-Delahaie, I.: Contribution à l’analyse physique et à la modélisation du fluage propre du béton.

Laboratoire Central des Ponts et Chaussées, Série Ouvrages d’Art OA25, Paris, 1997.

Guse U., Hilsdorf, H.K.: Surface Cracking of High Strength Concrete. Proc. of the 4th Weimar Workshop on High Performance Concrete, High Performance Concrete: Material Properties and Design, eds. F. H. Wittmann and P. Schwesinger, AEDIFICATIO Verlag, Freiburg und Unterengstringen, p. 69-89, 1995.

Guse, U., Hilsdorf, H.K.: Dauerhaftigkeit hochfester Betone. DAfStb Heft 487, Beuth Verlag GmbH, Berlin 1998.

Gutierrez, P. A., Canovas, M. F.: The modulus of elasticity of high performance concrete. Materials and Structures, Vol. 28, 1995, pp. 559-568.

Gylltoft, K.: A Fracture Mechanics Model for Fatigue in Concrete. Materials and Structures, Vol. 17, No. 97, 1984.

Hampel, T., Scheerer, S., Speck, K., Curbach, M.: High Strength Concrete under Biaxial and Triaxial Loading. Proceedings of the 6th International Symposium on Utilization of High Strength/High Performance Concrete, Vol. 2, Leipzig, Germany, 2002, pp. 1027-1036.

Han, N., Walraven, J. C.: Creep and Shrinkage of Young High Strength Concrete. Proc. of the 4th International Symposium on Utilization of High-Strength/High-Performance Concrete, Paris, France, pp. 339-348, 1996.

Han, N., Walraven, J.C.: Creep and shrinkage of high strength concrete. Progress in Concrete Research Vol. 5, Delft University of Technology, 1997, pp. 3-12.

Han, N., Walraven, J.C.: Sustained loading effects in high strength concrete. Proceedings High-Strength Concrete 1993, I. Holand and E. Sellevold eds., Vol. 2, Lillehammer, 1993, pp. 1076-1083.

Hansen, E. A., Leive, M., Rodriguez, J., Cather, R.: Mechanical Properties of High Strength Concrete - Influence of test Conditions, Specimens and Constituents. Proceedings of Fourth International Symposium on the Utilization of High Strength / High Performance Concrete, I. Holand and E.J.

Sellevold (eds.), Vol. 2, Paris, France, 1996, pp. 187-196.

Hansen, E. J., Hansen, K. K., Persson, B.: Concrete, hardened: Self-desiccation. Nordtest Procedure NT Build 490, NORDTEST OY, Espoo, Finland, 1999, 8 pp.

Haque, M. N., Kayali, O.: Properties of high-strength concrete using a fine fly ash. Cement and Concrete Research, Vol. 28, No. 10, 1998, pp. 1445-1452.

Hashin, Z.: Analysis of composite materials: A survey. Journal of Applied Mechanics, Vol. 16, 1983, pp. 481/505.

Heinrich, U., Seyfarth, K., Stark, J.: Dauerhaftigkeit von Hochleistungsbeton. DAfStb, 37.

Forschungskolloquium, Bauhaus-Universität Weimar, 1999, pp. 145-155.

Held, M.: Ein Beitrag zur Herstellung und Bemessung von Druckgliedern aus hochfestem Normalbeton (B 60 – B 125). Dissertation, Darmstadt, 1994.

Hillerborg, A.: Analysis of one Single Crack. in: Fracture Mechanics of Concrete. F. H. Wittmann, Elsevier Science Publishers, Amsterdam, 1983.

Hilsdorf, H. K: Concrete. In: Concrete Structures Euro-Design Handbook. Ernst & Sohn Verlag, Berlin, 1995.

Hilsdorf, H.K., Müller, H.S.: Concrete. In: Structural Concrete, CEB/FIB Manual Textbook: Textbook on Behaviour, Design and Performance, Volume 1, 1999.

Holmen, J.O.: Fatigue of Concrete by Constant and Variable Amplitude Loading. Division of Concrete Structures, Norwegian Institute of Technology, University of Trondheim, 1979.

Hordijk, D.A.: Local Approach to Fatigue of Concrete. Doctoral Thesis, Delft University of Technology, Delft, 1991.

Hu, X.-Z., Wittmann, F. H.: Experimental method to determine extension of fracture process zone.

Journal of Materials in Civil Engineering, Vol. 2, 1990, pp. 15-23.

Hussein, A., Marzouk, H.: Behavior of High-Strength Concrete under Biaxial Loading. Applied Science Technical Report Series, East Report No. 98003, Memorial University of Newfoundland, St. John’s, Canada, 1998.

Igarashi, S., Bentur, A., Kovler, K.: Autogenous shrinkage and induced restraining stresses in high-strength concretes. Cement and Concrete Research Vol. 30 (2000), pp. 1701-1707.

Immam, M., Vandewalle, L., Mortelmans, F.: Are current concrete strength tests suitable for high strength concrete? Materials and Structures, Vol. 28, 1995, pp. 384-391.

Ipatti, A.: Effect of size, shape and end conditions of test specimens on compressive strength of HSC.

Helsinki, 1992.

Iravani, S.: Mechanical properties of high-performance concrete. ACI Materials Journal, title No. 93-M47, September-October 1996, pp. 416-426.

Jaccoud, J. P., Farra, B., Leclercq, A.: Tensile Strength - Modulus of Elasticity - Bond - Tension Stiffening - Limit State of Cracking. Report to the Joint CEB/FIP Working Group on HSC/HPC.

IBAP, EPF Lausanne, March 1995.

Jensen, J. J.: Ductility of High Strength Concrete at High Rate Loading. 3rd International Symposium on Utilization of High Strength Concrete/High Performance Concrete, Lillehammer, 1993, pp.

241-250.

Jianyong, L., Pei, T.: Effect of slag and silica fume on mechanical properties of high strength concrete.

Cement and Concrete Research, Vol. 27, No. 6, 1997, pp. 833-837.

Karsan, I.D., Jirsa, J.O.: Behaviour of Concrete under Compressive Loads. Journal of the Structural Division, Vol. 95, Nr. ST12, 1969.

Kessler-Kramer, C., Diehl, K., Mechtcherine, V., Müller, H.S.: High Strength Concrete under Cyclic Tensile Loading. Proceedings of the 6th Int. Symposium on Utilization of High Strength/High Performance Concrete, Leipzig, 2002.

Kessler-Kramer, C., Mechtcherine, V., Müller, H.S.: Fracture Mechanical Assessment of Railway Superstructures made of Concrete. 11th International Conference on Fracture, Turin, Italy, 2005.

Kessler-Kramer, C.: Tensile Structural Behaviour of Concrete under Fatigue Loading (in German).

Series of the Institute of Concrete Structures and Building Materials, University of Karlsruhe, Vol. 49, 2002.

Khatri, R. P., Sirivivatnanon, V., Gross, W.: Effect of different supplementary cementitious materials on mechanical properties of high performance concrete. Cement and Concrete Research, Vol. 25, No. 1, 1995, pp. 209-220.

Khayat, H. K., Bickley, J. A., Hooton, R. D.: High-strength concrete properties derived from compressive strength values. Cement, Concrete and aggregates, ASTM, Vol. 17, No. 1, June 1995, pp. 126-133.

Khedr, S. A., Abou-Zeid, M. N.: Characteristics of silica-fume concrete. Journal of Materials in Civil Engineering, Vol. 6, No. 3, Aug. 1994, pp. 356-375.

Kim, J.-K., Kim, Y.-Y.: Experimental Study of the Fatigue Behavior of High Strength Concrete.

Cement and Concrete Research, Vol. 26, No. 10, 1996.

Kim, J.-K., Kim, Y.-Y.: Fatigue Crack Growth of High-Strength Concrete in Wedge-Splitting Test.

Cement and Concrete Research, Vol. 29, 1999.

König, G., Danielewicz, I.: Fatigue Strength of Reinforced and Prestressed Concrete Members with Comments on the Design Calculations According CEB-FIP Model Code 1990 (in German).

Deutscher Ausschuss für Stahlbeton, Nr. 439, Beuth Verlag, Berlin, 1994.

König, G., Remmel, G.: Tensile behaviour of high-strength concrete (HSC). Darmstadt Concrete, Vol.

7, pp. 247-256, 1992.

Kovler, K., Igarashi, S., Bentur, A.: Tensile creep behavior of high strength concretes at early ages.

Materials and Structures / Matériaux et Constructions, Vol. 32, June 1999, pp. 383-387.

Kupfer, H., Hilsdorf, H. K., Rüsch, H.: Behavior of concrete under biaxial stresses. ACI Journal, Vol.

66, No. 8, 1969.

L’Hermite R.G., Mamillan, M., Lefèvre C.: Nouveaux résultats de recherches sur la déformation et la rupture du béton. Annales de l'Institut Technique du Bâtiment et des Travaux Publics, Vol. 18, No. 207-208, p. 323-360; see also International Conference on the Structure of Concrete, Cement and Concrete Association, London, p. 423-433, 1965.

Lambotte, H., Taerwe L.: Fatigue of Plain High Strength Concrete subjected to Flexural Tensile Stresses. Proceedings, Utilization of High Strength Concrete, Stavanger, 1987.

Lan, S., Guo, Z.: Biaxial Compression Behaviour of Concrete under Repeated Loading. ASCE Journal of Materials in Civil Engineering, Vol. 11, No. 2, 1999.

Le Roy, R., De Larrard, F.: Creep and Shrinkage of High-Performance Concrete: The LCPC Experience. Proc. of the 5th RILEM Symposium, Creep and Shrinkage of Concrete, eds. Z. P.

Bažant and I. Carrol, E & FN Spon, London, pp. 499-504, 1993.

Le Roy, R., De Larrard, F., Pons, G.: The AFREM Code Type Model for Creep and Shrinkage of High Performance Concrete. Proc. of the 4th International Symposium on Utilization of High-Strength/High-Performance Concrete, Paris, France, pp. 387-396, 1996.

Lerner, A.: Zeit- und Temperatureinflüsse auf die mechanischen Eigenschaften von hochfestem Beton.

Vertieferarbeit, Institut für Massivbau und Baustofftechnologie, Universität Karlsruhe, 2000.

Maage, M., Smeplass, S., Johansen, R.: Long term strength of high strength silica fume concrete.

High-Strength Concrete, Second International Symposium, ACI, Weston T. Hester ed., 1990, pp.

399-408.

Maage, M.: Strength and heat development in concrete: Influence of fly ash and condensed silica fume. American Concrete Institute Special Publication SP-91, 1986, pp. 923-940.

Malhotra, V. M, Carette, G. G., Sivasundaram, V.: Role of silica fume in concrete: a review. In:

Advances in Concrete Technology, V. M. Malhotra (ed.), 1994, pp. 915-990.

Malvar, L., Crawford, E.: Dynamic increase factors for concrete. 28. DDESB seminar Orlando, Florida, 1998.

Markeset, G.: Failure of Concrete under Compressive Strain Gradients. Doktor Ingeniøraforhandling 1993:110, Institutt for Konstruksjonsteknikk, Norsge Tekniske Høgskole Trondheim. 1993.

Marzouk, H., Hussein, A.: Effect of curing age on high-strength concrete at low temperatures. Journal of Materials in Civil Engineering, August 1995, pp. 161-167.

Marzouk, H., Hussein, A.: Properties of high-strength concrete at low temperatures. ACI Materials Journal, technical paper, title No. 87-M19, March-April 1990, pp. 167-171.

Masuda, Y., Nakamura, S.: Experimental study on mix proportion and properties of high-strength concrete using high-blaine fly-ash. Conference on Utilization of HSC/HPC, 1999, pp. 1237-1243.

Mattock, A.: Shear transfer in concrete having reinforcement at an angle to the shear plane. ASCE Special Publication 42, “Shear in reinforced concrete”, Michigan 1974, pp. 17-42.

Mau, S.T., Hsu, T.C., PCI Journal, Vol. 33, No. 1, Jan/Feb. 1988, pp. 166-170.

Mechtcherine, V., Garrecht, H., Hilsdorf, H. K.: Effect of temperature and loading rate on fracture behaviour of concrete subjected to uniaxial tension. Fracture Mechanics of Concrete Structures, F. H. Wittmann (ed.), Aedificatio Publishers, 1995, pp. 719-728.

Mechtcherine, V., Müller, H. S.: Effect of the test set-up on fracture mechanical parameters of concrete. Fracture Mechanics of Concrete Structures, H. Mihashi and K. Rokugo (eds.), Aedificatio Publishers, 1998, pp. 377-386.

Mechtcherine, V., Müller, H. S.: Fracture mechanical and fractological investigations on normal and high strength concrete. Proceedings of the Fifth International Symposium on Brittle Matrix Composites, A. M. Brand, V. C. Li and I. H. Marshall (eds.), Woodhead Publishing Ltd./Cambridge - Bigraf/Warshaw, 1997, pp. 231-240.

Mechtcherine, V., Müller, H.S.: Fracture Mechanical, Fractological and Numerical Investigations on the Failure Mechanisms of HPC. Proceedings of the 6th Int. Symposium on Utilization of High Strength/High Performance Concrete, Leipzig, 2002.

Mechtcherine, V.: Fracture Mechanical and Fractological Investigation on the Crack Propagation in Concrete (in German). Series of the Institute of Concrete Structures and Building Materials, University of Karlsruhe, Vol. 40, 2000.

Meyer, J.: Ein Beitrag zur Untersuchung der Verformungsfähigkeit von Bauteilen aus Beton unter Biegedruckbeanspruchung. Doctoral thesis. Institut für Massivbau und Baustofftechnologie.

Universität Leipzig, 1998.

Mindess, S.: Relationships between Strength and Microstructure for Cement-Based Materials: An Overview. Materials Research Society Symposia, Proceedings, Vol. 42, 1984 pp. 54-68.

Mola, F., Pisani, M.A.: Creep Analysis of Non-Homogeneous Concrete, Proceedings of the Fifth International RILEM Symposium on Creep and Shrinkage of Concrete, Z. P. Bazant and I. Carol ed., E & FN Spon, London, 1993, pp. 597-602.

Mucha, S.: Determination of Crack Growth in Different High Strength Concretes caused by Fatigue Loading. LACER 8, University of Leipzig, 2003.

Müller, H. S., Küttner C. H.: Characteristics and Prediction of Creep of High Performance Concrete.

Proc. of the 4th Weimar Workshop on High Performance Concrete, High Performance Concrete:

Material Properties and Design, eds. F. H. Wittmann and P. Schwesinger , AEDIFICATIO Verlag, Freiburg und Unterengstringen, p. 145-162, 1995.

Müller, H. S., Küttner C. H.: Creep of High-Performance Concrete - Characteristics and Code-Type Prediction Model. Proc. of the 4th International Symposium on Utilization of High-Strength/High-Performance Concrete, Paris, France, p. 377-385, 1996.

Müller, H. S., Kvitsel, V.: Kriechen und Schwinden von Beton, Grundlagen der neuen DIN 1045 und Ansätze für die Praxis. In: Beton- und Stahlbetonbau 97, No. 1, pp. 8-19, 2002.

Müller, H.S., Rübner K.: High-Strength Concrete - Microstructural Characteristics and Related Durability Aspects. In: Durability of High-Performance Concrete, ed. H. Sommer, RILEM, Cachan, France, p. 23-37, 1995.

Müller, H. S., Hilsdorf, H. K.: Constitutive relations for structural concrete. CEB Bulletin d'Information No. 217, April 1993, pp. 17-65.

Nelson, E.L., Carrasquillo, R.L., Fowler, D.W.: Fatigue of High Strength Concrete subjected to Biaxial Compression. Proceedings, Utilization of High Strength Concrete, Stavanger, 1987.

Neville, A.: Water and concrete: a love-hate relationship. ACI Concrete-International, Vol. 22, No. 12, pp. 34-38, December 2000.

Nilsen, U.A., Monteiro, P.J.M.: Concrete: a three phase material. Cement and Concrete Research, Vol.

23, 1993, pp. 147-151.

Nilsson, L.-O.: Moisture Problems in Concrete Flooring. Report TVBM-3002. Lund Institute of Technology, Lund, 1977.

Nordisk Industrifysik AB, www.industrifysik.se.

Norwegian Standard NS 3473: Concrete Structures, Design Rules, 1989.

Ohlsson, U., Daerga, P.A., Elfgren, L.: Fracture Energy and Fatigue Strength of unreinforced Concrete Beams at normal and low Temperatures. International Conference on Fracture and Damage of

Ohlsson, U., Daerga, P.A., Elfgren, L.: Fracture Energy and Fatigue Strength of unreinforced Concrete Beams at normal and low Temperatures. International Conference on Fracture and Damage of

In document FIB-42 (Page 120-133)